Anomalous kinetics of lath martensite formation in ... · PDF file austenite to martensite...
Embed Size (px)
Transcript of Anomalous kinetics of lath martensite formation in ... · PDF file austenite to martensite...
General rights Copyright and moral rights for the publications made accessible in the public portal are retained by the authors and/or other copyright owners and it is a condition of accessing publications that users recognise and abide by the legal requirements associated with these rights.
Users may download and print one copy of any publication from the public portal for the purpose of private study or research.
You may not further distribute the material or use it for any profit-making activity or commercial gain
You may freely distribute the URL identifying the publication in the public portal If you believe that this document breaches copyright please contact us providing details, and we will remove access to the work immediately and investigate your claim.
Downloaded from orbit.dtu.dk on: Jul 16, 2020
Anomalous kinetics of lath martensite formation in stainless steel
Villa, Matteo; Hansen, Mikkel Fougt; Pantleon, Karen; Somers, Marcel A. J.
Published in: Materials Science and Technology
Link to article, DOI: 10.1179/1743284714Y.0000000709
Publication date: 2015
Document Version Peer reviewed version
Link back to DTU Orbit
Citation (APA): Villa, M., Hansen, M. F., Pantleon, K., & Somers, M. A. J. (2015). Anomalous kinetics of lath martensite formation in stainless steel. Materials Science and Technology, 31(11), 1355-1361. https://doi.org/10.1179/1743284714Y.0000000709
https://doi.org/10.1179/1743284714Y.0000000709 https://orbit.dtu.dk/en/publications/4cd4e478-20c9-400d-a9fa-1ab2fc030560 https://doi.org/10.1179/1743284714Y.0000000709
Anomalous kinetics of lath martensite formation in stainless steel
M. Villa1, M. F. Hansen2, K. Pantleon1 and M. A. J. Somers1
1. Department of Mechanical Engineering, Technical University of Denmark, DK 2800 Kongens Lyngby, Denmark
2. Department of Micro and Nanotechnology, Technical University of Denmark, DTU Nanotech, DK 2800 Kongens Lyngby, Denmark
ABSTRACT The kinetics of lath martensite formation in Fe–17.3 wt-%Cr–7.1 wt-%Ni–1.1 wt-%Al–0.08 wt-%C stainless steel was investigated with magnetometry and microscopy. Lath martensite forms during cooling, heating and isothermally. For the first time, it is shown by magnetometry during extremely slow isochronal cooling that transformation rate maxima occur, which are interrupted by virtually transformation free temperature regions. Microscopy confirms martensite formation after athermal nucleation of clusters followed by their time dependent growth. The observations are interpreted in terms of time dependent autocatalytic lath martensite formation followed by mechanical stabilisation of austenite during the transformation process.
Keywords: Phase transformation kinetics, Martensitic phase transformation, Stainless steel, Magnetometry
INTRODUCTION The kinetics of the austenite to martensite transformation in ferrous alloys is classified into two categories: athermal and isothermal.1 In the athermal case, the fraction of transformed product does not depend on time and increases instantaneously with increasing driving force for transformation. In the isothermal case, the transformation is time dependent. An alternative interpretation2,3 suggests that the athermal reaction is an extremely fast isothermal transformation, making the distinction between the two categories purely hypothetical. The kinetics of martensite formation is classified into isothermal and anisothermal.2 Anisothermal transformations apparently proceed ather-mally on cooling (i.e. with increasing the driving force for transformation), but continue isothermally upon inter-rupting the cooling.4,5
An additional category of the austenite to martensite transformation kinetics is burst kinetics,6 which is characterised by sharp transformation steps on cooling.7 In burst kinetics, autocatalytic nucleation of martensite results in the abrupt transformation of a part of the material in an instantaneous and irreproducible transformation event, a so called burst.7 A burst takes place within a millisecond.8 On the other hand, austenite to martensite transformation kinetics characterised by a series of alternating accelerations and decelerations of the trans-formation on cooling is considered an anomaly.3,7,9,10 Such anomalous transformation kinetics differs from burst kinetics for the reproducibility9,10 and the timescale of the transformation steps, which is in the range 1–104 s.
Martensite in iron based alloys can appear as lath or plate morphology.11 The present manuscript focuses on martensite with lath morphology. Lath martensite formation kinetics characterised by a series of alternating retardations and accelerations of the transformation on cooling was demonstrated recently and independently in Refs. 9 and 10. The transformation kinetics was referred to as unusual9 and anomalous,10 respectively. In
Ref. 12, where similar observations were reported, the transformation product was bainitic ferrite.13 Analogies and differences between the works in Refs. 9 and 10 are listed in the following.
In Ref. 9, a train of transformation rate maxima, i.e. a series of alternating retardations and accelerations of the transformation, was observed with dilatometry and calorimetry on cooling a Fe–Ni–Co–Mo maraging steel at a rate ranging from 0.2to2.5Kmin-1. Overall, the kinetics of martensite formation on cooling appeared to be controlled by the driving force for transformation (i.e. athermal character), but (partial) isothermal character was identified by a measurable effect of the cooling rate on the transformation steps. As a matter of fact, the transformation rate maxima were more pronounced the faster the cooling, while the temperature at which they were observed, as well as their number, was independent of the cooling rate.
In Ref. 10, a train of transformation rate maxima was observed with dilatometry during cooling of a Fe–Cr– Ni–Cu martensitic stainless steel at cooling rates ranging from 0.015 to 500 K min-1, and anomalous transforma-tion kinetics was observed in the cooling rate range 1.5–50 K min-1. As for Ref. 9, overall, the kinetics of martensite formation on cooling appeared controlled by the driving force for transformation, but (partial) isothermal character was identified by a measurable effect of the cooling rate on the transformation steps. Moreover, isothermal martensite formation was demonstrated on interrupting the cooling. These observations are consistent with anisothermal transformation kinetics. The number of transformation rate maxima depended on the cooling rate and was 12, 9, 6 and 5 for cooling rates of 1.5, 5, 15 and 50 K min-1 respectively. For a cooling rate up to 15 K min-1, the transformation rate maxima also became more pronounced the faster the cooling. Despite strong similarities in the observed transformation kinetics, the mechanisms proposed to explain the observed trains of transformation rate maxima were different for the systems investigated in Refs. 9 and 10.
In Ref. 9, the train of transformation rate maxima was interpreted as the result of the simultaneous formation of specifically oriented martensite blocks within packages, throughout the specimen. The formation of lath marten-site subdivides the austenite grains at different length scales.14–16 First, austenite grains are divided into packets. Each packet contains several parallel blocks of martensite laths. The individual laths represent the smallest level of subdivision. Hence, according to Ref. 9, during the evolution of the transformation, the units of martensite are distributed over the majority of the (prior) austenite grains. This hypothesis was verified in the surface region of the material by in situ optical microscopy.17
Conversely, in Ref. 10, the train of transformation rate maxima was interpreted as the result of the interplay between the driving force for thermally activated autocatalytic martensite formation and the counteracting mechanical stabilisation of the austenite (see below) during the transformation. Moreover, according to Ref. 10, the units of martensite are not distributed over the majority of (prior) austenite grains but are grouped in clusters, which nucleate independently, while their growth is thermally activated and extends over several (prior) austenite grains. This interpretation is based on previous work on the formation of lath martensite in a Fe–Cr–Ni–Al stainless steel,18 where clusters of martensite units were observed at the surface of the material together with numerous unaffected austenite grains. Moreover, two transformation rate maxima were revealed by magnetometry upon isochronal cooling of the material at 0.1K min-1.18
The interpretation of the transformation mechanism reported in Ref. 10 takes into account the effects of the transformation induced elastic (i.e. stress) and plastic strains introduced in martensite and surrounding austenite.19–22 Elastic and plastic strains are responsible for both the autocatalytic character of the transformation and the mechanical stabilisation of the austenite.8 Hydrostatic (elastic) stress reduces the driving force for the austenite to martensite transformation23–25 and consequently counteracts the continuation of martensite development26 (i.e. mechanically stabilises the austenite27). Conversely, shear stress thermodynamically promotes both (stress assisted)28 nucleation and growth29 of martensite and may yield autocatalytic behaviour.11,27,30 Plastic deformation by the introduction of dislocations in austenite counteracts the movement of an existing martensite/austenite interface